# Tear Strength Analysis of MDX4-4210 and A-2186 Silicones with Different Intrinsic Pigments Incorporated by Mechanical and Industrial Methods

Authors: Marcelo Coelho Goiato; Adhara Smith Nobrega; Emily Vivianne Freitas da Silva; Daniela Micheline dos Santos; André Pinheiro de Magalhães Bertoz; Mariana Vilela Sonego; Clovis Lamartine de Moraes Melo Neto
Journal: International Journal of Dentistry
 (2019)

---

## Abstract

Objective. The aim of this study was to evaluate the tear strength of MDX4-4210 and A-2186 silicones with different intrinsic pigments incorporated by mechanical and industrial methods, comparing nonaged and aged groups. Materials and Methods. Twenty-four groups were created according to the American Society for Testing and Materials D-624/type C, half nonaged and half aged (n = 10): bronze mechanical MDX4-4210, bronze industrial MDX4-4210, black mechanical MDX4-4210, black industrial MDX4-4210, pink mechanical MDX4-4210, pink industrial MDX4-4210, bronze mechanical A-2186, bronze industrial A-2186, black mechanical A-2186, black industrial A-2186, pink mechanical A-2186, and pink industrial A-2186. All specimens were submitted to tear strength analysis. Data were submitted to the ANOVA and Tukey test (p<0.05). Results. An increase in the tear strength values was observed only for the bronze and black MDX4-4210, comparing nonaged and aged silicones (p<0.05), regardless of the manufacturing method. There was a difference in all comparisons between MDX4-4210 and A-2186 silicones with the same pigment type (p<0.05), regardless of the manufacturing method. In all cases, there was no difference in the manufacturing method comparing the MDX4-4210 or A-2186 groups with the same pigment. Conclusion. Accelerated aging did not influence the tear strength in all aged A-2186 silicones and in aged pink industrial and mechanical MDX4-4210 silicones. The other MDX4-4210 groups had an increase in the results after aging. In all cases compared, the A-2186 groups had higher tear strength values than the MDX4-4210 groups. Mechanical and industrial methods can be used for silicone preparation, without changing the tear strength.


---

## Body

## 1. Introduction

Maxillofacial prostheses play a fundamental role in the rehabilitation of patients with deformities resulting from trauma, congenital origins, or surgical procedures [1–9]. Restoring a patient's appearance allows them to improve their self-esteem, helping them lead a normal life [4, 7, 8].Currently, most maxillofacial prostheses are made of silicone elastomers [8, 10]. These are the most accepted materials due to the ease of handling, chemical inertia, proper strength, durability, biocompatibility [4, 11, 12], flexibility, texture similar to that of the human skin, and heat stability. Additionally, these materials repel water, blood, and organic materials, thus eliminating bacterial colonization [8].The thin margins of silicone prostheses are usually glued to the patient's face using a medical adhesive. The thin margins of this type of prosthesis are susceptible to tearing as the prosthesis is removed from the attached facial tissue [4, 6]. In addition, maxillofacial prostheses can be retained by implants. For this, a layer of acrylic resin is adhered to the silicone to facilitate the bonding of the silicone to the implant. However, there is no good chemical adhesion between the silicone and the resin, which can result in the tearing of the silicone during the removal of the prosthesis [7].An increase in the tear strength of a silicone can promote an increase in the esthetic quality of the facial prosthesis since it allows the use of thinner margins, with greater possibility of elongation and lesser chance of rupture [4]. According to Rai et al. and Aziz et al., the most important property for maxillofacial prostheses is the tear strength, from a clinical point of view [4, 6].Silicone elastomers may be influenced by a variety of factors, such as intrinsic pigmentation [4], ultraviolet (UV) light [8, 10], and/or the manufacturing method (pigment incorporation method into silicone) [13]. When the pigment is mixed with silicone, bubbles may be incorporated into the material. These bubbles may influence the mechanical properties (e.g., tear strength) of a silicone [13]. The method for incorporating pigment into silicone can help minimize bubble incorporation [13]. Therefore, the study of methods of incorporating the intrinsic pigment to the silicone is very important for the durability of a facial prosthesis.The Silastic MDX4-4210 is an elastomer widely used for facial rehabilitation [14–16]. In the studies of Dootz et al., Sanchez et al., and Haug et al., the tear strength of MDX4-4210 silicone is compared with that of A-2186 silicone [10, 15, 17]. However, these comparisons did not evaluate the incorporation of different pigments and/or different methods of manufacturing of these materials. Therefore, the aim of this study was to evaluate the tear strength of MDX4-4210 and A-2186 silicones with different intrinsic pigments incorporated by mechanical and industrial methods, comparing nonaged and aged groups.


## 2. Materials and Methods

For this study, Silastic MDX4-4210 (Dow Corning Corporation Medical Products, USA) and A-2186 (Factor II, AZ, USA) silicones were prepared with the addition of intrinsic pigments. Bronze (Functional Intrinsic II–215, Factor II, USA) and black (Black Functional Intrinsic II–205, Factor II, USA) pigments specific for characterization of prostheses were used. In addition, a new pink pigment (Orbital Colors, Brazil) was tested. The pink pigment was formed by the union of yellow, red, and black pigments and white opacifier. All tested pigments had an organic origin and the white opacifier (TiO2) had a mineral origin.The silicones and pigments were weighed on a digital analytical balance (Adventurer, Ohaus Corporation, USA). Each pigment from Factor II (bronze and black) corresponded to 0.2% of the weight of its respective silicone [2]. For the pink pigment, the pigments that constituted it corresponded to 0.6% (white) [18], 0.122% (yellow), 0.03% (red), and 0.006% (black) [2] of the silicone weight.A total of 240 specimens were manufactured (Figures1(a) and 1(b)). The silicones were manipulated according to each manufacturer's instructions at a temperature of 23 ± 2°C [2, 8, 9, 12]. Half of the specimens were fabricated by the mechanical method of incorporating the intrinsic pigment to the silicone. For this, the pigment was manually mixed with the silicone for 15 seconds, followed by a vacuum spatulation at 425 rpm in a mechanical spreader (Polidental Ind. e Com. Ltda, Brazil) until the mass became homogeneous. Subsequently, the silicone was inserted into a metal matrix. The matrix was closed and submitted to 1 ton for 10 minutes. After this period, the silicone contained in the matrix was placed on a bench and exposed to the environment (29°C) for 72 hours, until the complete polymerization of the material. The other half of the specimens was fabricated at Orbital Colors using the industrial method of incorporating the intrinsic pigment to the silicone by means of a grinding machine (CHSG/3-Roll Mill, Chemieland, China). The pigment was mixed with the silicone in the machine. Then, the silicone was inserted into the matrix, following the same procedure as the previous method. In this method, the Deutsches Institut für Normung (DIN—53235) was used. Specimens were made in matrices with standard dimensions and had a 2 mm thickness (Figure 2).Figure 1
(a) Flowchart of MDX4-4210 specimens. (b) Flowchart of A-2186 specimens.
(a)
(b)Figure 2
Dimensions of specimens based on ASTM D-624 (type C).Twenty-four groups were created, half nonaged and half aged (n = 10): bronze mechanical MDX4-4210, bronze industrial MDX4-4210, black mechanical MDX4-4210, black industrial MDX4-4210, pink mechanical MDX4-4210, pink industrial MDX4-4210, bronze mechanical A-2186, bronze industrial A-2186, black mechanical A-2186, black industrial A-2186, pink mechanical A-2186, and pink industrial A-2186.The specimens were submitted to the accelerated aging test using an accelerated aging chamber (Equilam, Brazil) according to the American Society for Testing and Materials—Designation G53-96) [19]. The lamps (UVB 313, 40 Watts, Equilam, Brazil) emitted UVB light at a wavelength of 313 nm and irradiation of 0.49 W/m2/nm. Then, they were subjected to alternating periods of UVB light and condensation using oxygen-saturated distilled water, under conditions of heat and 100% humidity. Each aging cycle lasted 12 hours. In the first 8 hours, the temperature was maintained at 60 ± 3°C and the UV light was imputed onto the specimens. In the last 4 hours, the temperature was maintained at 45 ± 3°C and a condensation period occurred without light [2, 3, 8, 11]. The aging was performed for a total of 1008 hours, and the deterioration caused by rain, dew, and UV light from the sun was simulated [2, 3, 8, 11]. This period corresponded to approximately one year of prosthesis use [11]. The specimens that would not be aged were stored in a dark chamber at room temperature (23 ± 2°C) and 50 ± 5% relative humidity for 1008 hours [20].All specimens were tested using a universal testing machine (EMIC, Instron, Brazil) (Figure3). Specimens were stretched at a rate of 500 mm/min. The maximum tear strength value was recorded in Newtons (N). The process was determined according to the American Society for Testing and Materials (ASTM) D-624 (type C) [4, 14, 17]. The formula T = F/D was used, with F being the maximum force required to break the specimen and D being the thickness of the specimen. The results were obtained in N/mm.Figure 3
Specimen positioned for tear test.All data were analyzed using the Statistical Package for Social Sciences 20.0 (SPSS-IBM Corp., USA). The normal distribution was verified through the Shapiro–Wilk test. Data were analyzed through the analysis of variance (ANOVA) and the Tukey test, with a level of significance of 5%.


## 3. Results

Tables1–5 show the mean and standard deviation (SD) of each group. In Table 1, the tear strength of nonaged and aged silicone groups with the same pigmentation was compared. These comparisons were made within each manufacturing method. An increase in the tear strength values was observed only for the bronze and black MDX4-4210 silicone, for both manufacturing methods (p<0.05).Table 1
Mean values ± standard deviation (SD) (N/mm) of tear strength values comparing nonaged and aged silicones.
Manufacturing method
Pigment/Silicone
Nonaged groups
Aged groups
p value
Mean ± SD
Mean ± SD
Mechanical
Bronze A-2186
68.89 ± 7.74
72.12 ± 11.17
0.387
Bronze MDX4-4210
27.44 ± 2.45
41.16 ± 4.31
0.001∗
Black A-2186
63.79 ± 14.21
64.87 ± 13.91
0.773
Black MDX4-4210
29.40 ± 2.54
41.25 ± 3.82
0.002∗
Pink A-2186
63.11 ± 12.74
65.56 ± 12.83
0.513
Pink MDX4-4210
28.02 ± 7.64
31.65 ± 2.05
0.340
Industrial
Bronze A-2186
66.24 ± 9.99
73.10 ± 11.56
0.067
Bronze MDX4-4210
26.46 ± 1.86
37.82 ± 3.52
0.003∗
Black A-2186
67.81 ± 7.84
65.17 ± 11.85
0.484
Black MDX4-4210
29.49 ± 3.23
42.53 ± 6.66
0.001∗
Pink A-2186
69.18 ± 11.17
70.46 ± 6.07
0.722
Pink MDX4-4210
27.04 ± 1.07
31.06 ± 4.11
0.282
∗Statistically significant difference (p<0.05, Tukey).Table 2
Mean values ± standard deviation (SD) (N/mm) of tear strength values comparing nonaged MDX4-4210 and A-2186 silicones, based on same pigmentation.
Manufacturing method
Pigment
Silicone
Nonaged groups
p value
Mean ± SD
Mechanical
Bronze
MDX4-4210
27.44 ± 2.45
<0.001∗
A-2186
68.89 ± 7.74
Black
MDX4-4210
29.40 ± 2.54
<0.001∗
A-2186
63.79 ± 14.21
Pink
MDX4-4210
28.02 ± 7.64
<0.001∗
A-2186
63.11 ± 12.74
Industrial
Bronze
MDX4-4210
26.46 ± 1.86
<0.001∗
A-2186
66.24 ± 9.99
Black
MDX4-4210
29.49 ± 3.23
<0.001∗
A-2186
67.81 ± 7.84
Pink
MDX4-4210
27.04 ± 1.07
<0.001∗
A-2186
69.18 ± 11.17
∗Statistically significant difference (p<0.05, Tukey).Table 3
Mean values ± standard deviation (SD) (N/mm) of tear strength values comparing aged MDX4-4210 and A-2186 silicones, based on same pigmentation.
Manufacturing method
Pigment
Silicone
Aged groups
p value
Mean ± SD
Mechanical
Bronze
MDX4-4210
41.16 ± 4.31
<0.001∗
A-2186
72.12 ± 11.17
Black
MDX4-4210
41.25 ± 3.82
<0.001∗
A-2186
64.87 ± 13.91
Pink
MDX4-4210
31.65 ± 2.05
<0.001∗
A-2186
65.56 ± 12.83
Industrial
Bronze
MDX4-4210
37.82 ± 3.52
<0.001∗
A-2186
73.10 ± 11.56
Black
MDX4-4210
42.53 ± 6.66
<0.001∗
A-2186
65.17 ± 11.85
Pink
MDX4-4210
31.06 ± 4.11
<0.001∗
A-2186
70.46 ± 6.07
∗Statistically significant difference (p<0.05, Tukey).Table 4
Mean values ± standard deviation (SD) (N/mm) of tear strength values comparing mechanical and industrial methods of incorporation of pigments to nonaged MDX4-4210 and A-2186 silicones, based on same pigmentation.
Silicone
Pigment
Manufacturing method
Nonaged groups
p value
Mean ± SD
MDX4-4210
Bronze
Mechanical
27.44 ± 2.45
0.621
Industrial
26.46 ± 1.86
Black
Mechanical
29.40 ± 2.54
0.975
Industrial
29.49 ± 3.23
Pink
Mechanical
28.02 ± 7.64
0.784
Industrial
27.04 ± 1.07
A-2186
Bronze
Mechanical
68.89 ± 7.74
0.481
Industrial
66.24 ± 9.99
Black
Mechanical
63.79 ± 14.21
0.284
Industrial
67.81 ± 7.84
Pink
Mechanical
63.11 ± 12.74
0.105
Industrial
69.18 ± 11.17
∗Statistically significant difference (p<0.05, Tukey).Table 5
Mean values ± standard deviation (SD) (N/mm) of tear strength values comparing mechanical and industrial methods of incorporation of pigments to aged MDX4-4210 and A-2186 silicones, based on same pigmentation.
Silicone
Pigment
Manufacturing method
Aged groups
p value
Mean ± SD
MDX4-4210
Bronze
Mechanical
41.16 ± 4.31
0.364
Industrial
37.82 ± 3.52
Black
Mechanical
41.25 ± 3.82
0.739
Industrial
42.53 ± 6.66
Pink
Mechanical
31.65 ± 2.05
0.878
Industrial
31.06 ± 4.11
A-2186
Bronze
Mechanical
72.12 ± 11.17
0.789
Industrial
73.10 ± 11.56
Black
Mechanical
64.87 ± 13.91
0.932
Industrial
65.17 ± 11.85
Pink
Mechanical
65.56 ± 12.83
0.185
Industrial
70.46 ± 6.07
∗Statistically significant difference (p<0.05, Tukey).Table2 shows all nonaged groups, comparing MDX4-4210 and A-2186 silicones, based on the same pigment type. These comparisons were made within each manufacturing method. The tear strength values were higher for the A-2186, compared with the MDX4-4210 silicone (p<0.05).Table3 shows all aged groups, comparing MDX4-4210 and A-2186 silicones, based on the same pigment type. These comparisons were made within each manufacturing method. In all cases, the tear strength values were higher for the A-2186, compared with the MDX4-4210 silicone (p<0.05).Table4 shows all non-aged groups, comparing the mechanical and industrial methods, within the MDX4-4210 and A-2186 groups, with the same pigment type. There was no difference between the manufacturing methods (p>0.05).Table5 shows all aged groups, comparing the mechanical and industrial methods, within the MDX4-4210 and A-2186 groups, with the same pigment type. There was no difference between the manufacturing methods (p>0.05).


## 4. Discussion

In this study, it was possible to observe a statistically significant increase in the tear strength of aged bronze and black MDX4-4210 silicone, for both manufacturing methods, when compared with the respective nonaged groups. These results show that there was an increase in the tear strength of this silicone, regardless of the pigment color (lighter or darker). Presumably, the polymerization of this material was incomplete after its manufacture, and the UV light continued this process [8]. Despite this, there was no increase in this property for aged pink industrial and mechanical MDX4-4210 groups (Table 1). This could have occurred because the new pink pigment has TiO2 in its constitution. This component has a high refractive index and is used in the manufacture of sunscreens to protect human skin against UV rays [8, 11, 18]. Therefore, the TiO2 must have prevented UV rays from influencing the polymerization of pink industrial and mechanical MDX4-4210 groups.For the A-2186 groups, regardless of the pigment or manufacturing method, there was no significant statistical difference in tear strength comparing nonaged and aged groups (Table1). This suggests that the polymerization of this silicone has been complete since its manufacture. Therefore, the UV rays had an insignificant influence on the same.Regardless of the manufacturing method, the A-2186 silicone showed significantly higher tear strength values compared with the MDX4-4210 silicone, when the same pigment was used (Tables2 and 3). This difference could have occurred due to the higher filler loading and/or higher molecular weight of the dimethylsiloxane polymer from the A-2186 silicone [16]. Despite using different methodologies, this result corroborates the studies performed by Dootz et al. [10], Sanchez et al. [15], and Haug et al. [17]. According to Sanchez et al., higher values of tear strength of the A-2186 silicone compared with the MDX4-4210 silicone may clinically indicate higher prosthesis longevity [15].When comparing mechanical and industrial methods for each silicone with the same pigment, there was no statistically significant difference (Tables4 and 5). This may have occurred because these methods generated a similar homogeneous mixture between the silicone and pigment, with minimal and similar incorporation of bubbles during silicone handling. It is important to emphasize that the industrial method required a grinding machine and DIN standardization. In addition, the grinding machine and DIN standardization required trained professionals. These factors increase the final cost and production time of the prosthesis for the patient. Therefore, the use of the mechanical method can be more economically advantageous and faster.This study had the limitation of the evaluation of only one property (tear strength) in the facial silicones. Therefore, there is a need for other studies evaluating other properties.


## 5. Conclusion

Accelerated aging did not influence the tear strength in all aged A-2186 silicones and in aged pink industrial and mechanical MDX4-4210 silicones. The other MDX4-4210 groups had an increase in the results after aging. In all cases compared, the A-2186 groups had higher tear strength values than the MDX4-4210 groups. Mechanical and industrial methods can be used for silicone preparation, without changing the tear strength.



---

*Source: 2573095-2019-12-21.xml*